# Vegetal-FRCM Failure under Partial Interaction Mechanism
## 3 Results
### Meshes Tensile Test  
The results of the yarn meshes' tensile test can be found in Tables 7 and 8, where the average maximum load, peak displacement, maximum strength and strain at the peak are detailed. Moreover, [PERSON]'s modulus was calculated using linear regression. Both yarns were tested with all the possible coatings to select the ones for further research, where the maximum load (F\({}_{\text{peak}}\)) and peak displacement of the extensometer (\(\delta_{\text{peak}}\)) are detailed per specimen. Additionally, the maximum load, peak displacement of the extensometer, maximum strength (\(\sigma_{\text{peak}}\)), strain at peak (\(\epsilon_{\text{peak}}\)) and [PERSON]'s modulus (E) per case are detailed. Moreover, [PERSON]'s modulus was calculated using a linear regression of the \(\sigma\)-\(\epsilon\) curve. In order to calculate the strength, the cross-section of the yarn was used (21.20 mm\({}^{2}\) for cotton and 6.28 mm\({}^{2}\) for hemp). For the strain, the displacement was divided by the natural longitude of the extensometer (50 mm). Figures 6 and 7 show the average curves of the test for each yarn. The three repetition per case curves can be found on Supplementary materials in Figures S15-S22. \begin{table}
\begin{tabular}{c c c c c c c c c} \hline \hline \multirow{2}{*}{**Fiber**} & \multirow{2}{*}{**Coating**} & \multirow{2}{*}{**F\({}_{\text{peak (N)}}\)**} & \multirow{2}{*}{\(\delta_{\text{peak (mm)}}\)} & \multicolumn{6}{c}{**Average per Case**} \\ \cline{5-8}  & & & & \(\mathbf{F_{\text{peak (N)}}}\) & & \(\delta_{\text{peak (mm)}}\) & \(\begin{array}{c}\sigma_{\text{peak}}\\ (\text{MPa)}\end{array}\) & \(\varepsilon_{\text{peak (\%)}}\) & \(\mathbf{E}\) (MPa) \\ \hline \multirow{5}{*}{-} & \multirow{5}{*}{-} & 91 & 0.94 & & & & & & \\ \cline{2-10}  & & 84 & 0.78 & & 89 (5\%) & 0.90 (11\%) & 454 & 1.79 & 24,160 \\ \cline{2-10}  & & 93 & 0.90 & & & & & & \\ \cline{2-10}  & & 110 & 0.59 & & & & & & \\ \cline{2-10}  & & 114 & 0.72 & & 110 32\%) & 0.63 (10\%) & 560 & 1.26 & 41,252 \\ \cline{2-10}  & & 106 & 0.56 & & & & & & \\ \cline{2-10}  & & 103 & 0.42 & & & & & & \\ \cline{2-10}  & PES & 107 & 0.43 & & 111 (9\%) & 0.51 (20\%) & 585 & 1.10 & 51,561 \\ \cline{2-10}  & & 123 & 0.67 & & & & & & \\ \cline{2-10}  & & 94 & 0.50 & & & & & & \\ \cline{2-10}  & GA & 68 & 0.61 & & 76 (20\%) & 0.54 (13\%) & 387 & 0.90 & 31,013 \\ \cline{2-10}  & & 66 & 0.50 & & & & & & \\ \hline \multirow{5}{*}{GAU} & \multirow{5}{*}{69} & \multirow{5}{*}{69} & \multirow{5}{*}{69} & \multirow{5}{*}{0.61 (26\%)} & \multirow{5}{*}{350} & \multirow{5}{*}{1.21} & \multirow{5}{*}{26,724} \\ \cline{2-10}  & & 67 & 0.47 & & & & & & \\ \cline{2-10}  & & 70 & 0.56 & & & & & & \\ \cline{2-10}  & & 69 & 0.76 & & & & & & \\ \cline{2-10}  & & 71 & 0.54 & & & & & & \\ \cline{2-10}  & & 71 & 0.42 & & & & & & \\ \cline{2-10}  & & 70 & 0.32 & & & & & & \\ \hline \multirow{5}{*}{COLAC} & \multirow{5}{*}{105} & \multirow{5}{*}{0.61} & \multirow{5}{*}{95} & \multirow{5}{*}{12\%} & \multirow{5}{*}{0.55 (13\%)} & \multirow{5}{*}{486} & \multirow{5}{*}{1.09} & \multirow{5}{*}{40,921} \\ \cline{2-10}  & & 96 & 0.47 & & & & & & \\ \cline{1-1} \cline{2-10}  & & 105 & 0.61 & & & & & & \\ \cline{1-1} \cline{2-10}  & & 85 & 0.55 & & & & & & \\ \hline \hline \end{tabular}
\end{table} 
Table 6: Hemp yarns’ tensile test results.